Innovative Coating Developments Using a New, User Friendly HVOF and Metal Based Powders G. R. Heath*, A. Tremblay, P. Andersson Castolin Eutectic, Switzerland *E-mail: email@example.com A. Arizmendi Morquecho Advanced Materials Research Center, Monterrey, Mexico
Abstract The practical experience with the new Castolin Eutectic CJK5 High Velocity Oxy Fuel thermal spray unit has grown since its successful launch in 2011. It has many design features that simplify the user interface and servicing, but maintaining outstanding coating quality. The technical and practical features are described with detailed microstructural characterization of the resulting carbide based coatings using an established powder composition from several powder sources. With the recent development of a state-of-the-art metal powder manufacturing plant in Europe, highest quality â€œsatellite-freeâ€? metal powders can be manufactured. New selffluxing chemistries have been developed that are also low in Nickel and are designed to have good wear resistant properties. With the growing practical experience and parameter optimization, several innovative powders and coatings have been developed and are presented. Microstructural and mechanical properties and their relationship to processing parameters are presented. Introduction Since the launch of the TAFA JP5000 the High Pressure oxygen/kerosene HVOF system has grown in popularity and became an established technology in the thermal spray industry (Ref 1) for delivering high quality coatings and a reasonable operating cost. Over the years, a few other related systems have entered the market (Ref 2). These range from entry level units (which have expanded the market but are limited on quality and reproducibility) or higher end units with more focus on sophisticated control for OEM and aero applications. The later models have traded size and complexity for reproducibility, reliability and monitoring. However, there is a market demand for a high quality kerosene HVOF system, which has the advantages of portability, improved ease of use, lower operating costs (deposition efficiency, capital costs, reliability, reproducibility, consumables, etc.). HVOF portability has long been an important requirement and units
have been launched on the market (Ref 3). The newly launched Castolin Eutectic CJK5 unit meets these market demands and this publication will present the latest results of development work with the unit for a range of materials. In the end, it is the coating quality which is the important product resulting from the HVOF unit, optimized powder and optimized spray parameters. This paper will highlight the sensitivity of the coating characteristics to powder source, powder type and spray parameters. In the field of HVOF technology, several popular coatings have evolved, for example in the area of hard chrome replacement (Ref 4, 5) and these will be tested/optimized to establish the quality of CJK5 in delivering equivalent or better quality than the current technology. In addition to the established HVOF powders and coatings, there is a constant demand to develop new coatings with improved performance that also meet the changing commercial and environmental needs. Two such needs that have developed are to reduce the amount of nickel that is used in certain alloys (for cost, environmental and health issues), and also to develop alternative alloys that rely less on high carbides content (WC, CrC) to give good coating wear properties. One option is to use metallic-based self-fluxing alloys which are available most commonly with Ni-Cr-B-Si compositions (Ref 6) and have a hardness range typically between 35-60 HRC. There is a long tradition of successful applications of self-fluxing alloys in tough wear and corrosion environments, including boiler coating (Ref 7), oil, etc. applied and fused with a variety of technologies. Corrosion resistance of these alloys is particularly good due to the high nickel, chrome and closed porosity (Ref 8). Recently, ironbased self-fluxing alloys have been developed but are not widely known or used in the HVOF industry. Several compositions of self-fluxing alloys were manufactured in a new powder production plant using water-water and dry gas atomization. The latter has an advanced system to produce satellite-free particles.
HVO OF Spraying The HVOF unit: The CJK5 (Figure 1) is designed as an o interfface operaator friendly equipment wiith intuitive operator that creates repeaatable high quality q coatinngs. The HV VOF with touch scrreen proceess is controlled by an inttegrated PC w (Figuure 2). The spraying s can be done auttomatically orr in manuual mode and a full robot innterface includdes automatically contrrolled shutdoown. The CJK5 C has a high presssure combbustion chambber: up to 8 bar b (120 psi),, 250 kW pow wer, coaxxial oxy-fuel innjection for cllean burn withh minimal carb rbon depoosits. Radial poowder injectioon into the low w pressure reggion plus the converginng-diverging nnozzle gives hiigh quality, deense c and m mass thickk coatings. Hiigh accuracy mass flow control flow powder feedeer ensure repeeatability and control. 100m mm, mm, 200mm nozzles n are avvailable and were w used in the 150m tests..
mponents of G Gun, Figuure 1: Portablle Castolin CJJK5 core com Conssole with touchh screen and ppowder feederr.
T To ensure reliaable and safe operation therre is full dust sealing oof system andd a complete set of interloocks, the softw ware is ppersonalizable with usual US SB, Ethernet, RS232 interfaaces. R Real time dataa logging witth programmaable intervals system loogs the requirred parameterss and actual operating o paraameters, ggas and fuel fflows, powderr feeder speedds, chamber pressure p aagainst time annd also logs seequence eventss and faults. D Data log ooutput via cssv data form mat through U USB, serial port p or E Ethernet to enaable remote aanalysis. The ssystem also crreates a standard reportt after sprayinng. Metthodology E Experimental A Approach T Two separate ssets of tests w were performed for this papper. The fi first (PART A)) was with jusst one powder,, WC/10Co/4C Cr from oone manufactuurer. Then thee same powdeer batch was sprayed s w with the CJK5 with a set of 18 tests beingg performed, w which 3 sets of parameeters were varried to determ mine the sensitivity of thhe coating qquality and Deposition D Effficiency (DE E). The vvariables were a) spray nozzzle length, b) sspray distancee and c) fu fuel flow rate (ml/min). Thee exact param meters used are given inn Table 1. Thhe parameters that stayed fiixed during thhe trials aare given in Taable 2. T The second sett of tests (PAR RT B) used a standard set oof spray pparameters forr WC/10Co/44Cr compositiion powder, bbut this tiime 4 differennt powder supppliers were uused all offerring the same nominal composition and nominallly identical ppowder. O One of the pow wders, Powderr No. 4, was uused for 2 furthher sets oof tests with thhe CJK5. In thhese two tests tthe parameterrs of the C CJK5 were opttimized to obttain a lower poorosity coatingg. Once thhe lower poroosity level was achieved, thhese parameterrs were fu further optimizzed to create an â€œenhancedd optimized saampleâ€?. A All 4 powders were also sprrayed with a m market leadingg liquid fu fuel HVOF unnit with the ssame set of pparameters as for the C CJK5. All sam mples from thhe CJK5 andd the market leading liiquid fuel HVOF unit were processed in pparallel. T Table 1: Test cconditions andd variables in P PART A sprayy trials
Figuure 2: CJK5 ttouch screen control panell, for monitorring s of all pparameters duuring sprayingg and storage
Table 2: Fixed test conditions in PART A spray trials Powder Robot movement Substrate Spray Time Powder Feed
WC/10Co/4Cr Traverse: 300 mm/s Pitch: 5 mm S235JR (300 x 200 x 5 mm) 1.2 mins 80 g/min
Powder Samples All of the WC/10Co/4Cr powders that were sprayed were purchased from established manufacturers and suppliers of tungsten carbide HVOF powders. The metallic powders sprayed were manufactured at Castolin Eutectic Ireland Limited, in Dublin, Ireland which possesses a state-of-the-art gas-gas powder atomization tower, incorporating a novel design that can produce â€œsatellite freeâ€? metallic powders. These have better flow parameters, a lower specific surface area and have been shown to give better quality coatings and deposition characteristics over conventional metal powders. Scanning Electron Microscope (SEM) images of the powders are given in Figure 3, to show the difference between conventional and a satellite-free, metallic powder.
Advanced 3.2 image analysis software. The other method used was the water absorption method (Ref 9) performed at the Swedish research institute Swerea IVF AB. Microhardness: Microhardness on WC/Co/Cr samples was measured on polished cross sections on a Vickers hardness machine with a 300 g load (HV0.3). For the NiCrBSi and Febased self-fluxing coatings hardness was measured using a Vickers hardness machine with a 2 kg load (HV2). All values quoted are average values. Bond strength measurement: Bond strength was measured at the Swedish research institute Swerea IVF AB using the EN 582 procedure. Surface roughness measurement: The surface roughness of the samples in PART A trials was measured and standard Ra and Ry values were given in microns. Table 3: Test procedure overview Porosity Bond strength Coating thickness Hardness Flow ability Powder chemistry Particle size distribution DE% Powder feeding
Figure 3: SEM photos of metallic powders produced with conventional and satellite-free powder atomizer towers. Sample Preparation and Testing In Table 3 is an overview of the parameters used for analyzing the various coatings sprayed. Specific details are below. Sample preparation: Standard 300 x 200 x 5 mm S235JR mild steel plates were used for all tests. Prior to spraying they were grit blasted to remove all rust, oxide and any dirt. The sample was then weighed before and after spraying, and the amount of powder sprayed was also weighed before and after. Microscopy: After spraying the samples were sectioned using a Presi Mecatone T260 cut off machine, mounted and polished on a Presi Mecapol P230 polishing machine. All samples were studied in cross-section on a Leica DM4000M optical microscope. The samples were not etched. Porosity measurement: Coating porosity was measured by two distinctly different methods. One was with the polished cross section in the optical microscope using the Motic Images
Parameter optimization Temperature influence Surface roughness
Water absorption + image analysis EN 582 Micrometer and in optical microscope HV0.3 and HV2 Hall flow Induction Coupled Plasma JEL sieves EN ISO 17836 Weighing and ocular from gun Varying parameters Temperature measurement Ra and Ry
Results PART A An overview of the PART A trial results are given in Table 4, with the number of the sample corresponding to the spray conditions given in Table 1. What is clear is the large variation in the values of DE (%), hardness and surface roughness, and quite a poor correlation between the parameter in terms of quality. The best all-rounder appears to be sample 16, which offers a HV0.3 value of 1229 and a DE of 42% with one of the lowest Ra/Ry values. However even higher DE values were measured at 46% in 2 samples but at the expense of lower hardness values. The highest HV0.3 values of 1423 and 1351 were obtained but both at a DE of 32%.
Table 4: Test resullts overview fr from PART A trials. tr
RT B PAR An overview o of thhe PART B triial results are given in Figurre 4 for hardness meeasurements and Figure 5 for poroosity meassurements. Inn both Figures are includeed the additioonal “optiimization paraameter” whichh is seen in Sample No. 4 and the “enhanced “ opptimized sampple” found ass Sample No. 5. Bothh of these weree performed w with the powdeer Sample No. 4. WC//10Co/4Cr Allloys Harddness measureements: The reesults in Figurre 4 show thatt for all thhe 4 differentt suppliers off WC/10Co/4C Cr chemistry that the hhardness obtaained were alll above 1100 HV0.3, but w with Powdder No.4 giviing the higheest value of 11300 HV0.3 w with standdard parameteers. The hardnness values oobtained with the samee 4 powders ssprayed with the market leeading liquid ffuel HVO OF unit were generally sim milar +/- 100 HV0.3, in eitther direcction. Optimizzation of the P Powder No. 4 did not moddify the hardness siggnificantly w with the CJK K5. The highhest with the CJK55 in meassured hardnesss was howevver obtained w this sseries of trials.
pparameters. Foor the 4 powdders with the CJK5, all poorosities w were measuredd to be below w 2.3%. Withh the market leading liiquid fuel H HVOF unit the variatioon in the pporosity m measurements were even greeater, showingg a range from m 3.2 to 00.75%.
F Figure 5: Poorosity (%) values measuured for thee same ccomposition poowder from 4 different supppliers with sttandard C CJK5 spray paarameters (sam mples 1-4).
T The interestiing results came from m the optim mization eexperiments w with the Powdeer No. 4 and thhe CJK5. Heree it was ppossible to redduce the porossity level from m around 2% down d to 00.2% purely w with the changiing of spray pparameters. Thhis is an eexcellent levell of porosity aand the microsstructure is shhown at tw wo magnificattions in Figuree 6.
Figuure 4: Hardness HV0.3 vaalues measureed for the saame fferent supplieers with standdard compposition powdder from 4 diff CJK55 spray param meters (samplees 1-4). ments: The poorosity results in Figure 5 foor 4 Poroosity measurem diffeerent supplierss of WC/10Coo/4Cr chemistry show a laarge varieety of results. This could reflect the ssensitivity in the meassurement of porosity p at thhese low leveels, but also the criticcal effect onn porosity off powder suupply and sppray
F Figure 6: Polished P crosss-sections oof Sample 5, the W WC/10Co/4Cr chemistry with “ennhanced parrameter ooptimization” and low porossity.
Metaallic Alloys Harddness measureements: The hhardness of thhe NiCrBSi allloy sprayyed with the C CJK5 with 2 sets of differennt parameters w was recorrded at 30 andd 38, with the highest hardnness being relaated to thhe lower sprayy rates, which also gave the highest DE. T The Fe-based self fluxxing alloy wass sprayed andd a HRC valuee of 60 w was recorded. Poroosity measurements: For tthe NiCrBSi as sprayed w with non-optimized parrameters a first analysis of thhe microstructture gavee a 0.25% poroosity level. Thhe Fe-based allloy porosity w was also recorded at unnder 1%. DE m measurements: For the NiC CrBSi alloy as sprayed with the 2 setts of parameteers, both gavee very good D DE results of 65% 6 and 71%. This latter value is very v high for HVOF coatinngs. The DE for the F Fe-based self-ffluxing alloy was measuredd at 67% on the single test performedd. Table 5: NiCrSiB B Powder sprray parameterrs and measuured propperties. HRC values are convverted from H HV2 values.
Diiscussion T There are seveeral interestingg things that caame out of thiis work. F Firstly, the new w CJK5 HVOF unit has prooven that it is ccapable oof producing hhigh quality, reeproducible cooatings. The hardness vvalues of 13000 HV0.3 andd porosity leevels of 0.3% %, with m measured DE of up to 46% % for the WC//10Co/4Cr chemistry aalloy reflect this. The ddirect comparrison with iddentical ccoatings prodduced with thhe same pow wders on a leading ccomparable liqquid fuel HVO OF system, shhows superiorr results inn terms of porrosity and harddness. T The importancce of powder source was also demonstraated for eessentially ideentical powdders in termss of chemisttry and specification. The differeences were most signifficantly oobserved in thhe porosity measurement. m However, aan even bbigger differennce was obseerved when thhe CJK5 paraameters w were optimizedd in 2 stages for f a single powder, that of P Powder N No. 4. Here it was possible to reduce thee porosity level from aaround 2% doown to 0.2% ppurely with thhe changing oof spray pparameters. Att the same time the hardnness reduced slightly w with increasingg porosity. H However, if a correlation is sought bbetween hardnness and poroosity for the range r of paraameters, systems and powders in both A and B trials, noo clear ccorrelation cann be found. A stronger corrrelation betweeen DE aand hardness is found for WC/10Co/4C Cr powders (innverse). H However, the opposite was found for thee self-fluxing alloys, w where a directt increasing hardness was aachieved withh higher D DE. T The first resultts with the Nii- and Fe-baseed self-fluxingg alloys aare very promising in termss of their veryy low porosityy below 11% and high DE D above 65% %. Con nclusions
Figuure 7: Optical micrograph of o the CJK5 ssprayed Fe-baased self-ffluxing alloy powder. p Bondd Strength Meeasurements All W WC/10Co/4Crr coatings hadd their bond sttrength measuured accorrding to the EN E 582 standarrd and all sam mples failed in the adheesive which shhows that all coatings c had a minimum bond VOF strenngth of 71MPa, which iss typical forr quality HV coatiings today.
T The new CJK K5 HVOF unitt has proven that it is cappable of pproducing highh quality, reprroducible coatiings. The impportance oof the powder source for thee one alloy (W WC/10Co/4Cr) studied inn detail and shown to hhave an impportant effect.. More im mportant wass the effect oof parameter optimization on the pporosity of thiss coating. Thee first results oof HVOF spraaying of N Ni- and Fe-baased self-fluxiing metallic ppowders show wed DE leevels above 665% and poroosity below 1% %. The high D DE and cchemical/hardnness flexibilityy of these selff-fluxing alloyys could pprovide an addvantage over conventionall HVOF coattings in w wear and corroosion applicattions. The resuults for the Fee-based aalloys were encouraging and could be the bassis for ddevelopment of o lower costt, more ecoloogical coatinggs with eexcellent mechhanical properrties. The abovve results are jjust the ppreliminary woork on a new w system and also with som me new ppowders. The results will bbe repeated inn the on-goinng work pprogram to coonfirm sensitivvities of coatiing quality w with this system. Futurre work on the sensitivitty of DE, poorosity, hhardness and w wear results off these alloys aand others.
References 1. J.R. Davis, Introduction to HVOF Thermal Spray Processing Handbook of Thermal Spray Technology, ASMI and TSS 2004, p 3-13 2. R. Schwetzke and H. Kreye, Microstructure and Properties of Tungsten Carbide Coatings Sprayed with Various HighVelocity Oxygen Fuel Spray Systems, Journal of Thermal Spray Technology, Volume 8, Number 3, 433-439, September 1999 3. G.R. Heath, R.J.Dumola, M. Dvorak and R. Torday, Practical Experience with the New Generation of LowCost, Portable HVOFs, International Thermal Spray Society 1998, poster. 4. HCAT, “The Hard Chrome Alternatives Team Introduction to Thermal Spray Processing” http://www.hcat.org/about.html, Feb. 25, 2008 5. G. Bolelli, R. Giovanardi, L. Lusvarghi and T. Manfredini, Corrosion Resistance of HVOF-Sprayed Coatings for Hard Chrome Replacement, Corrosion Science, 2006, Vol. 48, Issue 11, p 3375-3397
6. M.P. Planche,, H. Liao, B. Normand and C. Coddet, Relationships between NiCrBSi Particle Characteristics and Corresponding Coating Properties Using Different Thermal Spraying Processes, Surface and Coatings Technology, Volume 200, Issue 7, 21 December 2005, Pages 2465–2473 7. G.R. Heath, R. Polak, T. Tsujita and S. Gustafsson, Role of Thermal Spray Coatings in Boilers; Development of Reliable Spray and Fuse Coatings for Boiler Protection, National Thermal Spray Society, 1996, p 1-8 8. G.R. Heath, P. Heimgartner, G. Irons, R. Miller and S. Gustafsson, An Assessment of Thermal Spray Coating Technologies for High Temperature Corrosion Protection, 4th International Conference on High Temperature Corrosion, Les Embiers (1996) 9. J. Skogsmo and P. Andersson, Comparison of Different Techniques for Porosity Measurements of Thermally Sprayed Coatings, MC International Metallography Conference, Colmar, France, 10-12 May 1995